View by Category

The presentation will start after a short

(15 second) video ad from one of our sponsors.

Hot tip: Video ads won’t appear to registered users who are logged in. And it’s free to register and free to log in!

(15 second) video ad from one of our sponsors.

Hot tip: Video ads won’t appear to registered users who are logged in. And it’s free to register and free to log in!

Loading...

PPT – Concrete mix design by PowerPoint presentation | free to download - id: 3bc27e-NzI1N

The Adobe Flash plugin is needed to view this content

About This Presentation

Write a Comment

User Comments (0)

Transcript and Presenter's Notes

WELCOME

CEMENT CONCRETE MIX DESIGN

by

K. RAMESH

Research Officer, Engineering Materials

Laboratory, A.P. Engineering Research

Laboratories, Himayatsagar, HYDERABAD-500030.

- Cement Concrete Mix Design means, determination

of the proportion of the concrete ingredients

i.e. Cement, Water, Fine Aggregate,Coarse

Aggregate which would produce concrete possessing

specified properties such as workability,

strength and durability with maximum overall

economy.

Methods of Concrete Mix Design

- I.S. Method
- British Method
- A.C.I. Method etc.

- These Methods are based on two basic assumptions
- Compressive Strength of Concrete is governed by

its Water-Cement Ratio - Workability of Concrete is governed by its Water

Content

- Data required for concrete mix design
- Grade of Concrete
- Eg RCC-M30-A20
- Slump required in mm
- Eg 25 75 mm
- Degree of Site Control
- Eg Good
- Type of Exposure
- Eg Moderate
- Grade of Cement
- Eg OPC 43 Grade

Workability (Clause 7.1, IS456-2000)

Degree of Site Control (Table 8, IS456-2000)

Type of Exposure (Table 3, IS456-2000)

- Approximate Quantity of Materials required for

concrete mix design - Cement 200 Kg.
- Fine Aggregate 240 Kg.
- Coarse Aggregate 180 Kg. (20 mm)
- 180 Kg. (10 mm)

- STEPS INVOLVED IN CONCRETE MIX DESIGN
- Step I- Determine the physical properties of
- concrete ingredients.
- I. CEMENT (OPC 43 Grade)

- FINE AGGREGATE
- 1. Sieve Analysis

2. Specific Gravity 2.60 3. Unit Weight in

Kg/Cu.m a) Loose 1460 b) Rodded 1580 4. Mat

erials Finer than 75 micron 1.00 3 Max ( by

weight)

III. 20.0mm COARSE AGGREGATE 1. Sieve Analysis

2. Specific Gravity 2.65 3. Unit Weight in

Kg/Cu.m a) Loose 1467 b) Rodded 1633

IV. MECHANICAL PROPERTIES

V. 10.0mm COARSE AGGREGATE 1. Sieve Analysis

2. Unit Weight in Kg/Cu.m a) Loose 1427 b) Rod

ded 1587

VI. BLENDING OF COARSE AGGREGATE

- Step II- Compute Target Mean Compressive

Strength

Fck fck t S Fck Target Mean

Compressive Strength at 28 days in

N/Sq.mm fck Characteristic

Compressive Strength at 28 days

in N/Sq.mm S Standard Deviation in

N/Sq.mm t A Statistic, depending on accepeted

proportion of low

results. 1.65 for 1 in 20

accepted proportion of low

results

Values of t

Assumed Standard Deviation (Table 8,

IS456-2000)

- Step III- Select the Water-Cement ratio of trial

mix from - experience

- Step IV- Select the water content per

cubic metre of - concrete from table2 of

I.S 10262-2009.

Approximate water content (Kg)

per cubic metre of concrete

(Table 32, SP23-1982)

Volume of Coarse

Aggregate per Unit Volume of

Total Aggregate (Table 3,

IS10262-2009)

- Step V- Compute the quantity of cement as

follows. - Water
- Cement -------------
- W/C Ratio
- 185 / 0.45

411 Kg.

Step VI- Then we find the quantities of

Fine Coarse aggregate by absolute volume method.

V (WC/Sc(1/p) (fa/Sfa)) (1/1000)

- (Eq.1) and V (WC/Sc(1/(1-p))

(ca/Sca)) (1/1000) - (Eq.2) Where V

Absolute volume of fresh concrete 1 m3 W

Mass of Water (Kg) per m3 of concrete C

Mass of Cement (Kg) per m3 of

concrete p Percentage of fine aggregate.

fa Mass of fine aggregate ca Mass of

coarse aggregate Sc Specific gravity of

cement. Sfa Specific gravity of fine

aggregate. Sca Specific gravity of coarse

aggregate.

- Substituting the values in Eq(1), we get
- 1000 185 411/3.0 (1/0.36) fa /2.6)
- 185 137 fa/0.936
- 322 fa/0.936
- fa (1000 322) 0.936
- 678 0.936
- 635 Kg.

- Substituting the values in Eq(2), we get
- 1000 185 411/3.0 (1/0.64) ca /2.65)
- 185 137 ca/1.696
- 322 ca/1.696
- ca (1000 322) 1.696
- 678 1.696
- 1150 Kg.

- So the mix proportion works out to be
- W C fa ca
- 185 411 635 1150
- 0.45 1 1.55 2.80
- This mix will be considered as Trial Mix No.2

- Step VII- Make slump trials to find out the

actual weight of water - to get required slump.

Make corrections to the water - content FA, if

required. - Step VIII- Compute 2 more trial mixes with W/C

ratios as 0.40 - 0.50, taking FA as

34 and 38 respectively.

- Trial Mix No. 1-
- Cement 185 / 0.4 462.5 Kg.
- Substituting the values in Eq(1), we get
- 1000 185 462.5/3.0 (1/0.34) fa /2.6)
- fa 584 Kg.
- Substituting the values in Eq(2), we get
- 1000 185 462.5/3.0 (1/0.66) ca /2.65)
- ca 1156 Kg.
- So the mix proportion works out to be
- W C fa ca
- 185 462.5 584 1156
- 0.4 1 1.26 2.50

- Trial Mix No. 3-
- Cement 185 / 0.5 370 Kg.
- Substituting the values in Eq(1), we get
- 1000 185 370/3.0 (1/0.38) fa /2.6)
- fa 683 Kg.
- Substituting the values in Eq(2), we get
- 1000 185 370/3.0 (1/0.62) ca /2.65)
- ca 1136 Kg.
- So the mix proportion works out to be
- W C fa ca
- 185 370 683 1136
- 0.5 1 1.85 3.07

- Step IX- Cast atleast 3 cubes for each trial

mix. - Step X- Test the cubes for compressive strength

at 28 days.

28 Days Compressive Strengths of Trial Mixes

- Step XI- Draw a graph between compressive

strength Vs C/W Ratio.

(No Transcript)

- Step XII- From the graph, find the W/C ratio for

the required - target mean compressive

strength. - Step XIII- Calculate the mix proportions

corresponding to - the W/C ratio, obtained

from the graph.

- Final Mix-
- From the graph, for a target strength of 390

Kg/Cm2, W/C ratio 0.47 - Cement 185 / 0.47 394 Kg.
- Substituting the values in Eq(1), we get
- 1000 185 394/3.0 (1/0.38) fa /2.6)
- fa 675 Kg.
- Substituting the values in Eq(2), we get
- 1000 185 394/3.0 (1/0.62) ca /2.65)
- ca 1123 Kg.
- So the mix proportion works out to be
- W C fa ca
- 185 394 675 1123
- 0.47 1 1.71 2.85

- Step XIV- Check the cement content W/C ratio

against the limiting values given in Table-5 of

I.S 456-2000 for given type of exposure type

of Concrete.

Table-5 Minimum Cement content Maximum

Water-Cement ratio and Minimum Grade of Concrete

for different exposures with normal weight of

aggregate of 20mm nominal maximum size.

From the table 5 of IS 4562000, the minimum

Cement content W/C ratio, For moderate, for RCC

are 300Kgs. 0.5 The Cement content 394Kgs.

gt 300Kgs. Hence Ok The W/C Ratio 0.47 lt 0.5

Hence Ok

TEST

REPORT Concrete Mix RCC M30 with 20.0mm M.S.A.

- Secondary Slides

Sieve Analysis of Fine Aggregate

- Weight of sample 500g (approx)
- Observations

Zones of Fine Aggregate

Sieve Analysis of Coarse Aggregate 2

20 mm aggregate a.

Minimum weight of sample 25 Kg

b. Observations

Sieve Analysis of Coarse Aggregate 2

10 mm aggregate a.

Minimum weight of sample 12 Kg

b. Observations

Target mean compressive strength

The value of S depends on Degree of Site

control and grade of concrete as given in I.S

4562000 (Table.8)

- Step IV-Fixation of Water Cement ratios for

trial mixes.

- Final Mix for RCC-M25-
- From the graph, for a target strength of 322

Kg/Cm2, W/C ratio 0.57 - which is gt 0.5, So, limit W/C ratio to 0.5

only. - Cement 185 / 0.5 370 Kg.
- Substituting the values in Eq(1), we get
- 1000 185 370/3.0 (1/0.38) fa /2.6)
- fa 683 Kg.
- Substituting the values in Eq(2), we get
- 1000 185 370/3.0 (1/0.62) ca /2.65)
- ca 1136 Kg.
- So the mix proportion works out to be
- W C fa ca
- 185 370 683 1136
- 0.50 1 1.85 3.07

Specific Gravity of Cement IS 4031

1988 Specific gravity of cement (Sc)

(W2 - W1) ----------------------------

x 0.79 (W4 - W1) - (W3 - W2) Where, W1

Weight of specific gravity bottle in g W2

Weight of specific gravity bottle with about

half filled cement in g W3 Weight of specific

gravity bottle with about half filled cement

rest is filled with

kerosene in g. W4 Weight of specific gravity

bottle completely filled with kerosene in g 0.79

Specific Gravity of Kerosene.

Specific Gravity of Fine Aggregate Coarse

Aggregate IS 2386 (Part.3) - 1963

D Specific gravity (Gs)

-------------- C ( A

B) Where, A Weight of Pycnometer

vessel containing sample filled with distilled

water in g B Weight of Pycnometer

completely filled with distilled water only in

g C Weight of saturated surface dry sample

in g D Weight of oven dried sample in g

(No Transcript)

Thank You

About PowerShow.com

PowerShow.com is a leading presentation/slideshow sharing website. Whether your application is business, how-to, education, medicine, school, church, sales, marketing, online training or just for fun, PowerShow.com is a great resource. And, best of all, most of its cool features are free and easy to use.

You can use PowerShow.com to find and download example online PowerPoint ppt presentations on just about any topic you can imagine so you can learn how to improve your own slides and presentations for free. Or use it to find and download high-quality how-to PowerPoint ppt presentations with illustrated or animated slides that will teach you how to do something new, also for free. Or use it to upload your own PowerPoint slides so you can share them with your teachers, class, students, bosses, employees, customers, potential investors or the world. Or use it to create really cool photo slideshows - with 2D and 3D transitions, animation, and your choice of music - that you can share with your Facebook friends or Google+ circles. That's all free as well!

For a small fee you can get the industry's best online privacy or publicly promote your presentations and slide shows with top rankings. But aside from that it's free. We'll even convert your presentations and slide shows into the universal Flash format with all their original multimedia glory, including animation, 2D and 3D transition effects, embedded music or other audio, or even video embedded in slides. All for free. Most of the presentations and slideshows on PowerShow.com are free to view, many are even free to download. (You can choose whether to allow people to download your original PowerPoint presentations and photo slideshows for a fee or free or not at all.) Check out PowerShow.com today - for FREE. There is truly something for everyone!

You can use PowerShow.com to find and download example online PowerPoint ppt presentations on just about any topic you can imagine so you can learn how to improve your own slides and presentations for free. Or use it to find and download high-quality how-to PowerPoint ppt presentations with illustrated or animated slides that will teach you how to do something new, also for free. Or use it to upload your own PowerPoint slides so you can share them with your teachers, class, students, bosses, employees, customers, potential investors or the world. Or use it to create really cool photo slideshows - with 2D and 3D transitions, animation, and your choice of music - that you can share with your Facebook friends or Google+ circles. That's all free as well!

For a small fee you can get the industry's best online privacy or publicly promote your presentations and slide shows with top rankings. But aside from that it's free. We'll even convert your presentations and slide shows into the universal Flash format with all their original multimedia glory, including animation, 2D and 3D transition effects, embedded music or other audio, or even video embedded in slides. All for free. Most of the presentations and slideshows on PowerShow.com are free to view, many are even free to download. (You can choose whether to allow people to download your original PowerPoint presentations and photo slideshows for a fee or free or not at all.) Check out PowerShow.com today - for FREE. There is truly something for everyone!

presentations for free. Or use it to find and download high-quality how-to PowerPoint ppt presentations with illustrated or animated slides that will teach you how to do something new, also for free. Or use it to upload your own PowerPoint slides so you can share them with your teachers, class, students, bosses, employees, customers, potential investors or the world. Or use it to create really cool photo slideshows - with 2D and 3D transitions, animation, and your choice of music - that you can share with your Facebook friends or Google+ circles. That's all free as well!

For a small fee you can get the industry's best online privacy or publicly promote your presentations and slide shows with top rankings. But aside from that it's free. We'll even convert your presentations and slide shows into the universal Flash format with all their original multimedia glory, including animation, 2D and 3D transition effects, embedded music or other audio, or even video embedded in slides. All for free. Most of the presentations and slideshows on PowerShow.com are free to view, many are even free to download. (You can choose whether to allow people to download your original PowerPoint presentations and photo slideshows for a fee or free or not at all.) Check out PowerShow.com today - for FREE. There is truly something for everyone!

For a small fee you can get the industry's best online privacy or publicly promote your presentations and slide shows with top rankings. But aside from that it's free. We'll even convert your presentations and slide shows into the universal Flash format with all their original multimedia glory, including animation, 2D and 3D transition effects, embedded music or other audio, or even video embedded in slides. All for free. Most of the presentations and slideshows on PowerShow.com are free to view, many are even free to download. (You can choose whether to allow people to download your original PowerPoint presentations and photo slideshows for a fee or free or not at all.) Check out PowerShow.com today - for FREE. There is truly something for everyone!

Recommended

«

/ »

Page of

«

/ »

Promoted Presentations

Related Presentations

Page of

Page of

CrystalGraphics Sales Tel: (800) 394-0700 x 1 or Send an email

Home About Us Terms and Conditions Privacy Policy Contact Us Send Us Feedback

Copyright 2016 CrystalGraphics, Inc. — All rights Reserved. PowerShow.com is a trademark of CrystalGraphics, Inc.

Copyright 2016 CrystalGraphics, Inc. — All rights Reserved. PowerShow.com is a trademark of CrystalGraphics, Inc.

The PowerPoint PPT presentation: "Concrete mix design by" is the property of its rightful owner.

Do you have PowerPoint slides to share? If so, share your PPT presentation slides online with PowerShow.com. It's FREE!